Peer-reviewed, accepted author manuscript of the following research article: Zhao, W., Given, M., Siew, W. H., Li, Q., & He, J. (Accepted/In press - 2019). Ageing Indices and Energy Delivery for Polymers Undergoing PD Activity Under Combined AC and DC Stress. IEEE Transactions on Dielectrics and Electrical Insulation, [8211].

**Ageing Indices and Energy Delivery for Polymers **

**Undergoing PD Activity Under Combined AC and DC **

**Stress **

**Weijia Zhao **

Global Energy Interconnection Research Institute Co. Ltd, State Key Laboratory of Advanced Power Transmission Technology,

Beijing 102211, China

**Wah Hoon Siew and Martin J Given **

University of Strathclyde
Department of Electronic & Electrical Engineering Glasgow G1 1XW, UK

**Qingmin Li **

North China Electric Power University Beijing Key Laboratory of High Voltage & EMC

Beijing, 102206, China

### and Jinliang He

Tsinghua University Department of Electrical EngineeringState Key Lab of Power Systems Haidian, Beijing 100084, China

**ABSTRACT **

**Samples of Polypropylene and High Density Polyethylene have been exposed to partial **
**discharge activity at elevated temperatures under the influence of combined AC and DC **
**stresses in the range of 1 and 2.5 kHz. Based on FTIR-ATR and dielectric spectroscopy **
**data values for the Carbonyl Index (CI), the low frequency conductivity (**0)** and a **
**proposed new index the Susceptibility Index (**I**) have been calculated to characterize the **
**degree of ageing in the samples. The Susceptibility Index reflects changes in the number **
**of dipoles and the distribution of dipole moments in the system as a result of ageing. The **
**rate of energy delivery from the partial discharge activity has also been calculated and **
**has been found to be dependent on the frequency of the AC component of the stress. **
**Strong correlations are observed between the behavior of the individual indices and the **
**rate of energy delivery. Possible reasons for these observed correlations are discussed **
**and the observed differences in the behavior of the ageing under different experimental **
**conditions are considered. **

Index Terms — partial discharge (PD), electrothermal aging, combined AC and DC aging, aging indices

**1 INTRODUCTION **

**T**

**HE**expected increases in the use of renewable energy sources such as photovoltaic cells and wind turbines has led to an increase in the requirements to transmit electrical power over long distances. This has led to an increase in the

importance of DC transmission systems due to their lower power losses and capital costs. [1, 2]. The operation of power electronic convertors and invertors leads to the injection of relatively high frequency harmonics (of the order of kHz) into the DC transmission system [3, 4]. There are reports that the combination of AC and DC stresses on polymer insulated cables can lead to changes in the ageing and degradation of the insulating system. [5, 6].

It is therefore important that the influence of a combination of AC. and DC stresses on the ageing of polymer insulation is assessed, and that any changes in the underlying mechanisms are identified to permit realistic estimation of insulation lifetime under these conditions. In [7] the authors reported results from an investigation of the behavior of High Density Polyethylene (HDPE) samples subjected to partial discharge activity under combined AC and DC stressing. The test geometry was chosen to model the ring cutting and slitting defects that can occur at cable terminations [8]. The data in [7] reported the general behavior of the phase resolved PD activity and the measured changes in the FTIR-ATR and dielectric spectra for HDPE samples. This paper analyses both the data reported in [7] and additional data on the behavior of Polypropylene (PP) in more detail: quantifying the energy dissipated in the partial discharges and the ageing of the polymers in terms of the Carbonyl Index [9]; changes in the dielectric susceptibility and in the low frequency (DC) conductivity of the material. The behavior of the phase resolved partial discharge activity as a function of the combined AC and DC stresses in PP was similar to that reported in [7] and can be seen in [10]

**2 EXPERIMENTAL METHODS **

A full description of the experimental system is given in
[7], so only the most significant details of the experimental
system are described here.
**2.1 ** **ELECTROTHERMAL AGEING SYSTEM **

The polymer materials, HDPE and PP were electrically stressed in a sphere plane gap at elevated temperatures in ambient air. The HDPE samples were tested at a temperature of 90C, which was just below the start of the melting peak for the material observed in Differential Scanning Calorimetry (DSC) thermograms. The PP samples were stressed at 90C to provide commonality with the HDPE tests but were also stressed at 110C, again a temperature just below the start of the melting peak.

The polymers came in the form of 50m films. It was
found, [7] that a single thickness of film was subject to bulk
breakdown under the conditions required for partial
discharge initiation. Therefore two samples of area of
6060mm2_{ were placed between the electrodes giving a total }

thickness of 100m. The upper, spherical, electrode was connected to a power amplifier with an output range of -50kV to + -50kV. The lower electrode was connected to ground with a current transformer (HFCT, type KH-100M) to detect and quantify the PD activity. Only the sample, which was in contact with the sphere electrode and had been exposed to the PD activity, was subjected to post ageing analysis. Further information on the test system is available in [7] and on the polymers used in [10].

**2.2 ** **AGEING CONDITIONS **

As the samples were subjected to a combination of AC and DC stresses, in [7] the authors specified the combined voltage waveform in terms of the frequency of the AC component and a Voltage Ratio (AC%):

𝐴𝐶% =𝑉𝐴𝐶

𝑉𝐷𝐶. 100 (1) where VAC is the peak value of the AC. component and VDC

is the DC voltage value. The quality of power system voltages under AC conditions is often described by the Total Harmonic Distortion (THD). An equivalent to THD can be defined for a combined AC and DC waveform in terms of the ratio of the powers associated with the AC and DC components.

𝑇𝐻𝐷𝐷𝐶=

(𝑉𝐴𝐶⁄√2) 2

𝑉𝐷𝐶 = 1 2(

𝑉𝐴𝐶 𝑉𝐷𝐶)

2

(2)
In this work, the DC voltage was kept constant at +6kV and
the values of *AC% *used were: 10%; 30% and 50%. The
equivalent levels of *THD*DC were: 0.005; 0.045 and 0.125

respectively. Four frequencies for the AC component were used: 1kHz; 1.5kHz; 2kHz and 2.5kHz.

The combination of AC and DC stressing resulted in surface discharge activity leading to the formation of a visibly degraded circular region centered on the point where the HV electrode was in contact with the surface. No measurable discharge activity occurred and no degradation was visible when the samples were exposed to pure DC stressing.

**2.3 ** **DIAGNOSTIC EQUIPMENT **

During the ageing process, the PD activity occurring on the surface of the sample was measured using a current transformer with a bandwidth of 2kHz to 120MHz connected to a computer controlled oscilloscope with a bandwidth of 1.5GHz and a sampling rate of 10GS/s (Yokogawa DL6154). During the one-hour sample ageing period, the activity for two complete cycles of the AC waveform component were recorded every 2.4 seconds. This resulted in a total of 1500 cycle pairs. Once data acquisition had been completed, the PD signals associated with the first of each pair of cycles were de-noised in Matlab to produce phase resolved partial discharge data (PRPD).

Changes in the samples after ageing were assessed using
FTIR-ATR and Dielectric Spectroscopy (DS) techniques.
The FTIR-ATR spectra were measured in the range of 350 cm
-1_{ to 4000 cm}-1_{ using a Thermos Fisher Nicolet iS 16 }

spectrometer. These measurements were performed on six
equally spaced regions of each sample at a radial distance of
1mm from the point of contact with the HV electrode, the
center of the aged area. Dielectric Spectra were measured on
samples with a diameter of 20mm again centered on the point
of contact between the HV electrode and the polymer, using
a Novocontrol Concept 82 spectroscopy system in the range
of 10-2 _{to 10}4_{ Hz. }

**3 AGEING PARAMETERS **

**3.1 ** **CUMULATIVE APPARENT ENERGY AND ITS **
**RATE OF DELIVERY **

For each PD pulse, the actual PD energy *E could be *
calculated from a measured voltage transient v*Meas(t) using: *

𝐸 =𝑅𝐷

𝑔 ∫ 𝑣𝑚𝑒𝑎𝑠(𝑡)𝑑𝑡 𝑇

0

(3)
Where *RD* is the resistance of the discharge channel,
assumed constant over the period of the discharge, g is
trans-resistance gain of the current transformer and *T is the pulse *
duration.

The total PD energy recorded during aging, E*CR*, will be a
summation of energy of each PD pulse recorded.

𝐸𝐶𝑅= 𝑅𝐷𝐸

𝑔 ∑ ∫ 𝑣𝑚𝑒𝑎𝑠(𝑡)𝑑𝑡 𝑇

0 𝑛

𝑘=1

(4)

where n is the number of pulses recorded and it is assumed
that a single effective discharge channel resistance R*DE* can
be used for all PD events.

If the shape of the individual PD pulses are broadly similar, then the integral term in the summation in (4) can be approximated by:

∫ 𝑣𝑀𝑒𝑎𝑠2 (𝑡)𝑑𝑡 𝑇

0

= 𝛽𝑇𝑘𝑣𝑘2 (5)

where * is a constant parameter depending on the assumed *
common shape of the partial discharges and v*k* and T*k* are the
peak voltage and duration associated with the discharge
event. If a final assumption is made that the period of the
individual PD events can be approximated by a common
effective period T*E*, Equation (4) can be rewritten as:

𝐸𝐶𝑅 = 𝑅𝐷𝐸

𝑔 𝛽𝑇𝐸∑ 𝑣𝑘2 𝑛

𝑘=1

(6)

As the term *g is constant and the terms RDE, * and T*E* are
assumed to be constant, the final summation term in (6)
should be proportional to the cumulative energy and is
referred to as the apparent cumulative energy E*CA*.

𝐸𝐶𝐴= ∑ 𝑣𝑘2 𝑛

𝑘=1

(7)

The data on partial discharge activity used by the authors came from 1500 cycles of the AC component of the voltage stress. The values of ECA calculated for different frequencies

are therefore based on different total periods of measurement
*TM*. Hence, the rate of apparent energy delivery P*CA* is a more
useful index for comparison

𝑃𝐶𝐴= 𝐸𝐶𝐴

𝑇𝑀 = 𝑓

1500𝐸𝐶𝐴 (8)

**3.2 ** **CARBONYL INDEX **

When polyolefin samples are aged, chain scission occurs
and subsequent reactions lead to the formation of hydroxyl
groups (O-H) and carbonyl groups (C=O) [11, 12]. This
leads to increases in absorption in FTIR-ATR spectra in the
region between 3500 cm-1_{ to 3000 cm}-1_{ for (O-H) groups and }

between 1750 cm-1_{ to 1600 cm}-1_{ for (C=O) groups. Peaks }

associated with the methylene group in the range of 2800 cm
-1_{ to 1600 cm}-1_{ and 1350 cm}-1_{ to 1480 cm}-1_{ will decrease as a }

result of these reactions. The Carbonyl Index (CI) attempts to quantify the degree of ageing by looking at the ratio of carbonyl absorbance to methylene absorbance. [11,12]

define the Carbonyl Index in terms of the carbonyl A*1720* and
the methylene A*1463* absorptions.

𝐶𝐼 =𝐴1720

𝐴1463 (9) This approach allows the ageing of a sample of polymer material to be in part quantified. However, while it is possible to use the CI calculated using Equation (9) to compare the degree of ageing of samples of a single polymer, it is not possible to directly compare the CI values of differing polymers.

**3.3 ** **LOW FREQUENCY OR DC CONDUCTIVITY **

As reported in [7, 10] at frequencies below 1Hz a rise in
tan was observed as the frequency decreased for aged
sample of HDPE, while the value of /_{ though dependent on }

the ageing conditions, was constant. This behavior can be
attributed to DC conduction processes [13]. Under all ageing
conditions the plots of //_{ against 1/}_{}_{ were linear in the low }

frequency range allowing values of the dc conductivity 0 to

be obtained.

**3.4 ** **PERMITTIVITY AND SUSCEPTIBILITY INDEX **

In [7, 10] the real part of the relative permittivity was
observed to increase as a function of ageing. As a way of
quantifying such changes, the authors have defined a
Susceptibility Index (*I): *

𝜒𝐼 =𝜒𝐴− 𝜒𝑈

𝜒𝑈 (10) Where U is the value of the dielectric susceptibility measured for an unaged sample and Ais that measured for a particular ageing condition. Dielectric susceptibility quantifies the relationship between the polarization density

**P** and the electric field vector **E** in a material. **P** and therefore
the value of will depend on the population, in terms of the
type and number per unit volume, of dipoles in a sample and
the dipole moment for each type of dipole. During ageing
dipoles with a low moment such as methyl groups are
replaced with dipoles with a higher dipole moment such as
carbonyl groups. This index therefore represents the change
in the polarization density due to the change in the dipole
distribution due to ageing, normalized by the original
polarization density.

**4 DERIVED PARAMETER VALUES **

Based on the partial discharge data, values for the
apparent power delivery P*CA*were calculated. The dielectric spectra were used to calculate values for the conductivity 0

and the susceptibility index *I. The FTIR ATR spectra were *
used to calculate values for the carbonyl index CI.

**4.1 ** **RATE OF APPARENT ENERGY DELIVERY **

The derived values of P*CA * at AC%30 and AC%50 for HDPE

conditions. The values of P*CA* are significantly higher for the
AC%50 tests as compared to the AC%30 tests. This reflects

the differences in the partial discharge activity reported in
[7]. For the samples stressed at AC%10 the values of P*CA* are
again lower. As there were little or no change in the values
of 0, I and CI for this voltage ratio these results are not

presented in this paper.

[image:4.612.355.526.55.179.2]**Figure 1 (a).** Rate of apparent energy delivery vs. frequency of AC
component for HDPE aged at 90C: □ 30% voltage ratio, ∆ 50% voltage
ratio.

**Table 1.**Mean of recorded PD voltages and their standard deviation for PP
samples aged at 110C [10]

Material, Temperature AC% Gradient (P*CA*/kHz) R2

HDPE, 90C 30% _{50% } 1.08 ± 0.01 _{9.20 ± 0.2 } _{0.999 }1.00

PP, 90C 30% _{50% } 0.84 ± 0.01 _{7.29 ± 0.21 } _{0.998 }1.00

PP, 110C 30% _{50% } 1.37 ± 0.08 _{10.8 ± 0.32 } 0.991 _{0.997 }

**4.2 ** **CARBONYL INDEX **

The behavior of the calculated values of CI as the
frequency of the AC component was varied are shown in
Figure 2. The A*1720* peak was not present in unaged HDPE
and PP samples or in samples exposed to only a DC stress,
therefore CI had a value of zero for these conditions. For the
HDPE sample at 90C and the PP sample at both 90 and
110C for AC%30 stressing, CI appears to increase in a

linearly with the frequency of the AC component.

The values calculated for CI are larger for the PP samples but as mentioned above, direct comparisons of the CI values calculated for different materials are not valid.

. The values of CI in each experimental condition are higher for AC%50 than for AC%30 and again the value of the

CI increases with the frequency of the AC component. For HDPE samples aged at 90C and PP samples aged at 110C some saturation of the value of CI can be observed at higher frequencies. Possible explanations for this behavior are discussed in section 5.4

**Figure 2(a).** Carbonyl Index vs. frequency of AC component for HDPE
aged at 90C: □ 30% voltage ratio, ∆ 50% voltage ratio.

**Figure 2(b).**Carbonyl Index vs. frequency of AC component for PP aged
at 90C: □ 30% voltage ratio, ∆ 50% voltage ratio.

**Figure 2(c).**Carbonyl Index vs. frequency of AC component for PP aged
at 110C: □ 30% voltage ratio, ∆ 50% voltage ratio.

**4.3 ** **LOW FREQUENCY CONDUCTIVITY **

### 0

**.**

For unaged samples the value of 0 was 1.37 0.14 10-16

S/m for HDPE and 2.06 0.19 10-16 _{S/m for PP. }

**Figure 3(b).** Conductivity vs. frequency of AC component using 50%
voltage ratio: □ HDPE at 90C, ◊ PP at 90C, ∆ PP at 110C

Figure 3a shows the behavior of 0as a function of the frequency of the AC component for HDPE and PP samples stressed at AC%30. The values of conductivity at 0 Hz are

those obtained from samples stressed only with DC voltage. It can be seen that 0 increases with the frequency of the AC component. The derived values of 0 for PP aged at 110C are greater for those for PP aged at 90C.

For the samples aged at AC%50, Figure 3b, the values of

0 derived are significantly higher in each case than those for AC%30. The relationship between 0 and the frequency of the

applied AC component is linear.

Again the values of 0 for PP samples aged at 110C are higher than those aged at 90C.

**4.4 ** **SUSCEPTABILITY INDEX ****I **

For all experimental conditions no significant structures
were observed in the / _{spectra in the range of 10}1_{ to 10}4_{ Hz. }

Therefore, an average value over this range was used to
calculate the value of the susceptibility. From the definition
of the susceptibility index (10), the value of *I for unaged *
samples will be zero. The behavior of the susceptibility index
as a function of the frequency of the AC component for the
various ageing conditions for the HDPE and PP material are
shown in Figure 4. The values of *I at 0 Hz were based on *
the derived values of for samples aged in the absence of an
AC voltage component. In Figure 4 for both the HDPE and
the PP samples the susceptibility index increases with the
frequency of the AC voltage component in a linear manner.

**Figure 4(a).** Susceptibility Index I vs. frequency of AC component using
30% voltage ratio: □ HDPE at 90C, ◊ PP at 90C, ∆ PP at 110C.

**Figure 4(b).**Susceptibility Index I vs. frequency of AC component using
50% voltage ratio: □ HDPE at 90C, ◊ PP at 90C, ∆ PP at 110C.

The changes in the *I for samples which were aged at *
AC%50 are larger than those for samples aged at AC%30. For

the PP samples, the changes in *I are larger for the samples *
aged at 110C as compared to those aged at 90C.

**5 COMPARISON OF INDEX **

**BEHAVIOURS AND DISCUSSION **

**5.1 ** **COMPARISONS BETWEEN AGING INDICES **

### 0

**AND**

###

**I**

Figure 5a shows a plot of 0 vs *I for the HDPE *
samples aged at 90 at AC%30 and AC%50. The values for

AC%50 appears to fall close to a linear trend. (R2 = 0.979).

The points associated with the AC%30 data fall

significantly below the trend-line for the AC%50 data

**Figure 5(a).** Conductivity vs. Susceptibility Index I for HDPE at
90C: ◊ 30% voltage ratio; ∆ 50% voltage ratio

**Figure 5(b).** Conductivity vs. Susceptibility Index I for PP aged at
50% voltage ratio open symbols 90C, closed symbols 110C

Figure 5b shows the data for the PP samples aged at AC%50

[image:5.612.359.528.57.178.2] [image:5.612.82.252.65.191.2] [image:5.612.334.503.393.510.2] [image:5.612.355.525.553.667.2] [image:5.612.80.250.563.687.2]and *I (R*2_{ = 0.981).As with HDPE the data for AC%}
30 for

both temperatures lies considerably below the trend associated with theAC%50 data and has been omitted from

Figure 5b for clarity. This behavior suggests that are significant differences for both polymers, between the ageing processes that occurs at AC%50 and AC%30, with the latter

resulting in a much smaller change in the low frequency conductivity as compared with the changes in susceptibility index.

**5.2 ** **COMPARISONS BETWEEN ****I, **

### 0

**INDICES**

**AND CI**

As there are linear relationships between the DC conductivity 0 and the susceptibility index I at AC%50

comparisons will only be made between the Susceptibility
Index and Carbonyl Index. in this section as no significant
additional information is obtained by comparisons with the
DC conductivity. It can be seen in Figure 6 that the
relationship between CI and *I is non- linear and empirical *
trendlines of the form:

𝐶𝐼(𝐼) = 𝐴(1 − exp(−𝐵(𝐼 −𝐼𝑑𝑐))) (11) have been fitted to the data as this provides the simplest analytical form for a saturation behavior. 𝐼𝑑𝑐 is the value of the susceptibility index for samples that were aged under only DC stress. For HDPE the data for both AC%30 and

AC%50% falls close to a common exponential trend line. For

PP the data for AC%50 at both 90 and 110C falls close to a

single trend line.

**Figure 6(a).** Carbonyl Index vs. Susceptibility Index for HDPE at
90C: ◊ 30% voltage ratio; ∆ 50% voltage ratio.

**Figure 6(b).** Carbonyl Index vs. Susceptibility Index for PP: open
symbols aged at 50%, closed symbols aged at 30% voltage ratio open
symbols 90C, closed symbols 110C. ◊ 90C; ∆ 100C.

Though it should be noted from Figure 4 b that the value of 𝐼𝑑𝑐 is different for the two ageing temperatures. The data for PP aged at AC%30 falls distinctly above this trend line,

suggesting that under these conditions the Carbonyl Index increases more rapidly compared to the Susceptibility index.

**5.3 ** **RELATIONSHIP BETWEEN AGING INDICES **
**AND APPARENT POWER **

Based on Equations (3) to (8) estimates were made of the
rate at which energy was being dissipated in the partial
discharge activity during ageing for the various stressing
conditions considered. Figure 7 shows the relationship of I
relating to changes in the polymer due to aging and *PCA*
which relates to the total energy supplied to the system
during aging. In Figure 7a it can be seen that the data points
for HDPE aged at 90C for both AC%30 and AC%50 have a

common linear behavior with respect to *PCA*(.R2 = 0.971).

For the PP data shown in Figure 7(b) for the samples aged at 110C there is again a common linear behavior for both AC%30 and AC%50 (R2 = 0.975). For the PP samples aged at

90C the data obtained at AC%50 follows a linear trend (R2 =

0.945). The data at AC%30 however falls above this trend

line. It is not shown in Figure 7b as it is superimposed on the AC%30 data for 110C. As would be expected due to the

strong linear correlation between 0 and the *I similar *
behaviors exist in the relationship between 0 and *PCA* at
AC%50.

The relationships between the derived Carbonyl Index and the apparent power delivered to the discharges for HDPE aged at 90 C are shown in Figure 8a The AC%50 data is

non-linear with the rate of increase in Carbonyl Index decreasing as the apparent power delivery increases. The data can be fitted to an exponential function of the form of Equation (11). The data for HDPE aged at AC%30 falls above this line of fit

**Figure 7(a).** Susceptibility Index vs P*CA* for HDPE at 90C: ◊ 30%

voltage ratio; ∆ 50% voltage ratio.

**Figure 7(b).** Susceptibility Index vs P*CA*for PP ◊ 30% voltage ratio; ∆

. A similar behavior is seen for the PP data in Figure 8b. The AC%50 data at 110C can again be fitted to (11). A fit to

this function for AC%50 data at 90C is also possible but the

fit is less good. For both the 90 and 110C the AC%30 data

falls above the fit lines for the corresponding AC%50 data.

**Figure 8(a)**Carbonyl Index vs. apparent power for HDPE aged at 90C:
◊ 30% voltage ratio, ∆ 50% voltage ratio.

**Figure 8(b)** Carbonyl Index vs. apparent power for PP: ◊ 30% voltage
ratio, ∆ 50% voltage ratio; Open symbols aged at 90C, closed symbols
aged at 110C.

**5.4 ** **DISCUSSION **

From the data it is not possible to separate the effects of
thermal ageing and the effects of pure DC stressing. No
partial discharge activity was observed in the DC stressed
samples, so any changes are expected to be due to thermal
ageing. Pure DC stress does not lead to changes in the
Carbonyl Index. For HDPE the value of 0 increased from
1.37 0.14 10-16_{ S/m to 6.57}_{}_{ 0.07 }_{}_{10}-16_{ S/m. For PP the }

values of 0* increased from 2.06* 0.18 10-16_{ S/m to 3.47}_{}

0.88 10-16_{ S/m at 90}_{}_{C and to 10.3}_{}_{ 0.02 }_{}_{10}-16_{S/m at }

110C. The values of *I has a value of 0.07 for the HDPE *
exposed to DC stress at a temperature of 90C. For PP it is 0
for DC stress at 90C but increases to 0.07 at 110C. Looking
at the data for combined DC and AC stressing at a frequency
of 2.5 kHz under AC%30 conditions the additional change in

0 and are *I of the same order of magnitude as any effect of *
thermal and DC aging. Under AC%50 conditions the changes

observed as a result of stressing are much more significant than the effect of combined DC and thermal stress.

For samples aged at AC%50 there are strong linear

correlations between 0 and *I. There are also linear *
correlations between these indices and the rate of apparent
energy delivery to the system *PCA*. The discharge activity
onto and across the surface of the polymer provides energy
to the system in the form of electrons, ions, active species

and high- energy (UV) photons. This results in changes in the morphology and structure of the polymer, which can lead to the formation of new trapping sites or the reduction in the depth of the traps already present in the system [14-16]. This would lead to increases in 0: firstly through the increase in the number of charge carriers within the system due to the increase in the available trapping sites and secondly through the higher average mobility of the charge carriers due to reductions in the average trap depth. Oxidative reactions are also taking place in the polymer due to the partial discharge activity [17-19] leading to the presence of more polar groups such as the carbonyl group in the polymer increasing its polarizability and therefore leading to an increase in the values of the susceptibility index. These oxidative processes will also result in significant changes in the IR spectra. [7, 10] as have been quantified through the Carbonyl Index.

If it is assumed that, at a constant temperature, the rate at
which these modifications to the polymer morphology,
structure and chemical composition will occur depends on
the rate of energy delivery to the surface from the discharge
activity. This assumption implies that over the period of the
ageing process the concentration of unreacted/unaged
polymer remains near constant. The rate of energy delivery
will increase as the power supplied by the discharge activity
increases leading to a corresponding increase in the aging of
the polymer. This would result in the observed correlations
between 0 and *I with PCA*.

The nonlinear behavior of the CI data when compared to
the behavior of 0 and *I may result from the limited *
penetration depth of the evanescent wave employed by FTIR
ATR spectroscopy at the point of total reflection. The
amplitude of this wave decays exponentially and the
penetration depth into a polymer is of the order of some
microns [20]. As the chemical reactions induced by the
discharge activity on the surface progress, the changes in
chemical composition and physical structure in the surface
layer accessible by FTIR ATR are likely to approach an
equilibrium state. As ageing continues, the chemical and
physical structure of the polymer in the region below this
surface layer will start to change. These changes in the bulk
of the polymer will lead to continuing changes in the values
of 0 and *I as they are derived from bulk dielectric *
spectroscopy measurements while the FTIR ATR spectra
remains unchanged leading to a saturation in the value of CI

The behavior of the results obtained when the samples were stressed at AC%30 are more difficult to explain. The

value of CI appears to be rising more rapidly as a function of
*PCA* than is the case for samples stressed at AC%50. This

behavior is also observed for *I for PP aged at a temperature *
of 90C. When comparing the correlation between 0 and *I *
the behavior in HDPE and the PP samples show a significant
difference between the relationships observed at AC%30 and

AC%50. A possible explanation comes from the approach

[image:7.612.83.251.130.249.2] [image:7.612.78.251.281.396.2]AC%50 tests. The currents for the AC%30 tests are therefore

significantly lower than those for the corresponding AC%50

tests. From the behavior of channel resistance proposed in
[21, 22], higher values of average channel resistance should
occur for the discharges with lower currents. This would lead
to higher values of the parameter R*DE* in Equation (5) for the
AC%30 discharge activity, so the values of P*CA* at AC%30 may

have been under-estimated. This would have the effect of moving the AC%30 data points in Figures 7 and 8 closer to

the fit lines for the AC%50 data. However an underestimate

in the value of *PCA* does not explain the difference in the
relationship between 0 and *I observed at AC%*30. This

suggests that while the energy of the discharges is still sufficient to cause the formation of polar groups, the energy is such that modification to the polymer structures and morphology occur at a much reduced rates.

**6 CONCLUSIONS **

Partial discharge based ageing experiments have been performed using combinations of DC and AC stressing on HDPE and PP polymer films. The degree of ageing of the polymers depends on both the magnitude of the AC component of the voltage and on its frequency. The effects of ageing on the polymer have been quantified using 3

parameters: the DC conductivity 0; a proposed

Susceptibility Index *I, both derived from dielectric *
spectroscopy data and the Carbonyl Index derived from
FTIR-ATR spectroscopy data. For the ageing conditions
using a 50% voltage ratio there are strong correlations
between 0 and *I. Correlations between these parameters *
may also exist at the 30% voltage ratio but the
proportionality between the parameters is different.

When comparing the Carbonyl Index with the parameters extracted from the dielectric spectroscopy data a clear saturation behavior was observed for CI at higher degrees of ageing. This reflects the fact that FTIR-ATR detects changes within a few microns of the polymer surface unlike dielectric spectroscopy, which detects changes in the bulk of the sample. The results indicate that as the sample ages the damage extends into the bulk to the polymer.

A simple method of estimating the apparent power delivered to the partial discharges, PCA, has been presented.

Despite the assumptions made, linear correlations exist between the derived values of PCA and the parameters 0 and

*I for the 50% stressing condition. The approach appears to *
be appropriate as long as the mean and distribution of the
partial discharge magnitudes are similar.

The ageing conditions reported in this paper were extreme,
in service conditions, the voltage ratio is unlikely to exceed
10% and no significant ageing was observed at this voltage
during the one hour tests performed. Longer tests at lower
values of voltage ratio are required to determine the life
surface as a function of voltage ratio. It will also be necessary
to determine the relationship of the derived parameters 0
and *I with a parameter such as breakdown strength directly *
related to the residual life of the materials.

**REFERENCES **

[1] L. Xu, L. Yao and C. Sasse, “Grid integration of large DFIG-based wind farms using VSC transmission,” IEEE Trans. Power Syst., vol. 22, no. 3, pp. 976-984, Aug. 2007.

[2] P. Bresesti, W. L. Kling, R. L. Hendriks and R. Vailati, “HVDC connection of offshore wind farms to the transmission system,” IEEE Trans. Energy Convers., vol. 22, no. 1 pp. 37–43, Mar. 2007. [3] C. Guo, Y. Zhang, A. M. Gole and C. Zhao, “Analysis of dual-infeed

HVDC with LCC–HVDC and VSC–HVDC,” IEEE Trans. on Power Del., vol. 27, no. 3 pp. 1529-1537, Jul. 2012.

[4] C. H. Chien and R. W. G. Bucknall, “Analysis of harmonics in subsea power transmission cables used in VSC–HVDC transmission systems operating under steady-state conditions,” IEEE Trans. Power Del., vol. 22, no 4; pp. 2489-2497, Oct. 2007.

[5] H. H. Sæternes, J. Aakervik and S. Hvidsten, “Water treeing in XLPE insulation at a combined DC and high frequency AC Stress,” IEEE Int.Conf. Electr. Insul. (ICEI), pp. 494-498, 2013.

[6] F. Mauseth, M. Amundsen and H. Faremo, “Water tree growth of wet XLPE cables stressed with DC and high frequency AC voltage superimposed,” IEEE Int. Conf. Electr. Insul. (ICEI), pp. 266–269, 2012.

[7] W. Zhao, W. H. Siew, M. J. Given, E. Corr, Q. Li and J. He “ Assessment of HDPE aged under DC voltage combined with AC harmonic stresses of various Frequencies,” IEEE Trans. on Dielectr. Electr. Insul., vol. 24, no.2 pp. 1189-1196, Apr. 2017.

[8] W. Vahlstrom, “Strategies for field testing medium voltage cables,” IEEE Electr. Insul. Mag., vol. 25, no. 5, pp. 7–17, Sept. 2009. [9] L. Barbeş , C. Rădulescu , C. Stihi, “ATR-FTIR spectrometry

characterisation of polymeric materials”, Romanian Rep. Phys., Vol. 66, No. 3, P. 765–777, 2014

[10] W. Zhao “Partial discharge ageing of polymer insulation under combined AC and DC stress at elevated temperatures,”, Ph.D. Thesis, University of Strathclyde, Glasgow, UK, 2017.

[11] E. Chiellini, A. Corti, S. d’Antone and R. Baciu, “Oxo-biodegradable carbon backbone polymers-Oxidative degradation of polyethylene under accelerated test conditions,” J. Polym. Degrad. Stab., vol.91, no. 11 pp. 2739-2747, Nov. 2006.

[12] E. Strömberg, S. Karlsson, “The design of a test protocol to model the degradation of polyolefins during recycling and service life”, J. App. Polym. Sci, vol.112, issue. 3, pp.1835-1844, 2009.

[13] A. K. Jonscher, “A new understanding of the dielectric relaxation of solids,” J. Mat. Sci., vol.16, no.8, pp.2037-2060, 1981.

[14] T. Zhou, G. Chen, R Liao, and Z. Xu “Charge trapping and detrapping in polymeric materials: Trapping parameters,” J. App. Phys., vol. 110, no. 4, pp. 043724, Aug. 2011.

[15] V.A. Goldade, L.S. Pinchuk, A.G. Kravtsovand and S.V. Zotov “TSD-study of Polyethylene photochemical degradation,” Proc. 2004 Int. Conf. on Solid Dielectr. (ICSD), France, pp. 347-350 , 2004. [16] G. Mazzanti ; G.C. Montanari ; J.M. Alison, “A space-charge based

method for the estimation of apparent mobility and trap depth as markers for insulation degradation -theoretical basis and experimental validation,” IEEE Trans. on Dielectr, and Electr. Insul., vol. 10, no. 2 pp. 187-197, Apr. 2003.

[17] L.A. Dissado and J.C. Fothergill, “Electrical degradation and breakdown in polymers,”. Peter Peregrinus-IEE. 1992

[18] P.H. Morshuis, “Degradation of solid dielectrics due to internal partial discharge: some thoughts on progress made and where to go now,” IEEE Trans. on Dielectr. and Electr. Insul. vol. 12, no. 5 pp. 905 - 913: Oct. 2005

[19] A. Tidjani, “Comparison of formation of oxidation products during photo-oxidation of linear low density polyethylene under different natural and accelerated weathering conditions,”, J. Polym. Degrad. Stab. vol. 68, no. 3pp 465–469, May 2000.

[20] J. D. Schuttlefield and V. H. Grassian “ATR–FTIR Spectroscopy in the Undergraduate Chemistry Laboratory. Part I: Fundamentals and Examples,” J. Chem. Educ., vol. 85, no. 2, p 279-288, Feb. 2008R [21] Rompe and W. Weizel, “Uber das Toeplershe Funkengesetz,” Z.

Physicz, vol. 122, pp. 636-639 1944